LMucko/crystallography-open-database huggingface dataset:
Crystal structure and physical properties of new ternary silicides R4 T13 X9 (R, rare earth or uranium; T, rhodium or iridium; X, silicon or germanium)
Verniere, A; Lejay, P; Bordet, P; Chenavas, J; Tholence, J L; Boucherle, J X; Keller, N; Journal of Alloys Compd. 218 (1995) 197–203; doi:10.1016/0925-8388(94)01400-0

data_1008678
_publ_section_title
;
Crystal structure and physical properties of new ternary silicides R4
T13 X9 (R, rare earth or uranium; T, rhodium or iridium; X, silicon or
germanium)
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              197
_journal_page_last               203
_journal_paper_doi               10.1016/0925-8388(94)01400-0
_journal_volume                  218
_journal_year                    1995
_chemical_formula_structural     'Er4 Ir13 Si9'
_chemical_formula_sum            'Er4 Ir13 Si9'
_chemical_name_systematic        'Erbium iridium silicide (4/13/9)'
_space_group_IT_number           59
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2c 2bc'
_symmetry_space_group_name_H-M   'P n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   18.84799(300)
_cell_length_b                   10.918(2)
_cell_length_c                   3.9153(5)
_cell_volume                     805.7
_refine_ls_R_factor_all          0.023
_cod_original_sg_symbol_H-M      'P n m m Z'
_cod_database_code               1008678
Crystal structure and physical properties of new ternary silicides R4 T13 X9 (R, rare earth or uranium; T, rhodium or iridium; X, silicon or germanium)
Verniere, A; Lejay, P; Bordet, P; Chenavas, J; Tholence, J L; Boucherle, J X; Keller, N; Journal of Alloys Compd. 218 (1995) 197–203; doi:10.1016/0925-8388(94)01400-0

data_1008679
_publ_section_title
;
Crystal structure and physical properties of new ternary silicides R4
T13 X9 (R, rare earth or uranium; T, rhodium or iridium; X, silicon or
germanium)
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              197
_journal_page_last               203
_journal_paper_doi               10.1016/0925-8388(94)01400-0
_journal_volume                  218
_journal_year                    1995
_chemical_formula_structural     'Ce Ir3 Si2'
_chemical_formula_sum            'Ce Ir3 Si2'
_chemical_name_systematic        'Cerium iridium silicide (1/3/2)'
_space_group_IT_number           74
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      74
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.1838(2)
_cell_length_b                   9.7373(3)
_cell_length_c                   5.6018(2)
_cell_volume                     391.9
_refine_ls_R_factor_all          0.089
_cod_database_code               1008679
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008680
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Mn0.1)2 D2.46'
_chemical_formula_sum            'Cr1.8 D2.46 Mn0.2 Zr'
_chemical_name_systematic
;
Zirconium chromium manganese deuteride (1/1.8/0.2/2.46)
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.381(3)
_cell_length_b                   5.381(3)
_cell_length_c                   8.798(6)
_cell_volume                     220.6
_refine_ls_R_factor_all          0.051
_cod_original_formula_sum        'D2.46 Cr1.8 Mn.2 Zr'
_cod_database_code               1008680
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008681
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Fe0.1)2 D3.66'
_chemical_formula_sum            'Cr1.8 D3.66 Fe0.2 Zr'
_chemical_name_systematic
;
Zirconium chromium iron deuteride (1/1.8/0.2/3.66)
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.374(2)
_cell_length_b                   5.374(2)
_cell_length_c                   8.784(4)
_cell_volume                     219.7
_refine_ls_R_factor_all          0.049
_cod_original_formula_sum        'D3.66 Cr1.8 Fe.2 Zr'
_cod_database_code               1008681
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008682
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Co0.1)2 D3.615'
_chemical_formula_sum            'Co0.2 Cr1.8 D3.615 Zr'
_chemical_name_systematic
;
Zirconium chromium cobalt deuteride (1/1.8/0.2/3.62)
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.370(2)
_cell_length_b                   5.370(2)
_cell_length_c                   8.789(3)
_cell_volume                     219.5
_refine_ls_R_factor_all          0.04
_cod_original_formula_sum        'D3.615 Co.2 Cr1.8 Zr'
_cod_database_code               1008682
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008683
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Ni0.1)2 D3.525'
_chemical_formula_sum            'Cr1.8 D3.525 Ni0.2 Zr'
_chemical_name_systematic
;
Zirconium chromium nickel deuteride (1/1.8/0.2/3.53)
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.367(2)
_cell_length_b                   5.367(2)
_cell_length_c                   8.793(3)
_cell_volume                     219.3
_refine_ls_R_factor_all          0.032
_cod_original_formula_sum        'D3.525 Cr1.8 Ni.2 Zr'
_cod_database_code               1008683
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008684
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Cu0.1)2 D3.684'
_chemical_formula_sum            'Cr1.8 Cu0.2 D3.684 Zr'
_chemical_name_systematic
;
Zirconium chromium copper deuteride (1/1.8/0.2/3.68)
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.357(2)
_cell_length_b                   5.357(2)
_cell_length_c                   8.722(3)
_cell_volume                     216.8
_refine_ls_R_factor_all          0.023
_cod_original_formula_sum        'D3.684 Cr1.8 Cu.2 Zr'
_cod_database_code               1008684
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008685
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr Cr2 D3.51'
_chemical_formula_sum            'Cr2 D3.51 Zr'
_chemical_name_systematic        'Zirconium chromium deuteride (1/2/3.51)'
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.680(2)
_cell_length_b                   7.680(2)
_cell_length_c                   7.680(2)
_cell_volume                     453.0
_refine_ls_R_factor_all          0.041
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'D3.51 Cr2 Zr'
_cod_database_code               1008685
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008686
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Mn0.1)2 D3.80'
_chemical_formula_sum            'Cr1.8 D3.8 Mn0.2 Zr'
_chemical_name_systematic
;
Zirconium chromium manganese deuteride (1/1.8/0.2/3.80)
;
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.754(2)
_cell_length_b                   7.754(2)
_cell_length_c                   7.754(2)
_cell_volume                     466.2
_refine_ls_R_factor_all          0.037
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'D3.8 Cr1.8 Mn.2 Zr'
_cod_database_code               1008686
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008687
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Fe0.1)2 D3.65'
_chemical_formula_sum            'Cr1.8 D3.65 Fe0.2 Zr'
_chemical_name_systematic
;
Zirconium chromium iron deuteride (1/1.8/0.2/3.65)
;
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.6551(8)
_cell_length_b                   7.6551(8)
_cell_length_c                   7.6551(8)
_cell_volume                     448.6
_refine_ls_R_factor_all          0.028
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'D3.65 Cr1.8 Fe.2 Zr'
_cod_database_code               1008687
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1- x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
Soubeyroux, J L; Bououdina, M; Fruchart, D; Pontonnier, L; Journal of Alloys Compd. 219 (1995) 48–54; doi:10.1016/0925-8388(94)05019-8

data_1008688
_publ_section_title
;
Phase stability and neutron diffraction studies of Laves phases Zr (Cr1-
x Mx)2 with M =Mn,Fe,Co,Ni,Cu and 0 < x <0.2 and their hydrides
;
_journal_coden_ASTM              JALCEU
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              48
_journal_page_last               54
_journal_paper_doi               10.1016/0925-8388(94)05019-8
_journal_volume                  219
_journal_year                    1995
_chemical_formula_structural     'Zr (Cr0.9 Co0.1)2 D3.56'
_chemical_formula_sum            'Co0.2 Cr1.8 D3.56 Zr'
_chemical_name_systematic
;
Zirconium chromium cobalt deuteride (1/1.8/0.2/3.56)
;
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.6605(7)
_cell_length_b                   7.6605(7)
_cell_length_c                   7.6605(7)
_cell_volume                     449.5
_refine_ls_R_factor_all          0.032
_cod_original_sg_symbol_H-M      'F d -3 m Z'
_cod_original_formula_sum        'D3.56 Co.2 Cr1.8 Zr'
_cod_database_code               1008688
Magnetic and structural properties of new Sm Co9 Si2 Cx compounds (x=0.,0.6,0.9)
Skolozdra, R; Akselrud, L; Fruchart, D; Gignoux, D; Gorolenko, Yu; Soubeyroux, J L; Tomey, E; Journal of Magnetism and Magnetic Materials 140 (1995) 915–916; doi:

data_1008689
_publ_section_title
;
Magnetic and structural properties of new Sm Co9 Si2 Cx compounds
(x=0.,0.6,0.9)
;
_journal_coden_ASTM              JMMMDC
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              915
_journal_page_last               916
_journal_volume                  140
_journal_year                    1995
_chemical_formula_structural     'Sm Co9 Si2 C0.6'
_chemical_formula_sum            'C0.6 Co9 Si2 Sm'
_chemical_name_systematic        'Samarium cobalt silicon carbide (1/9/2/0.6)'
_space_group_IT_number           141
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.838
_cell_length_b                   9.838
_cell_length_c                   6.377
_cell_volume                     617.2
_cod_depositor_comments
;
 Correcting the summary chemical formula by changing it from 'Co9 Si2 Sm'
 to 'C0.6 Co9 Si2 Sm'.

 Antanas Vaitkus,
 2018-07-07
;
_cod_original_sg_symbol_H-M      'I 41/a m d Z'
_cod_database_code               1008689
Low-temperature studies of two Y-type hexagonal ferrites: Ba Zn Fe6 O11 and Ba Co Fe6 O11
Collomb, A; Muller, J; Argoud, R; Journal of Magnetism and Magnetic Materials 130 (1994) 367–376; doi:10.1016/0304-8853(94)90696-3

data_1008690
_publ_section_title
;
Low-temperature studies of two Y-type hexagonal ferrites: Ba Zn Fe6 O11
and Ba Co Fe6 O11
;
_journal_coden_ASTM              JMMMDC
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              367
_journal_page_last               376
_journal_paper_doi               10.1016/0304-8853(94)90696-3
_journal_volume                  130
_journal_year                    1994
_chemical_formula_structural     'Ba0.98 Zn0.94 Fe5.905 O11'
_chemical_formula_sum            'Ba0.98 Fe5.905 O11 Zn0.94'
_chemical_name_systematic        'Barium zinc iron(III) oxide (1/1/6/11)'
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   5.861(1)
_cell_length_b                   5.861(1)
_cell_length_c                   43.50299(300)
_cell_volume                     1294.2
_refine_ls_R_factor_all          0.092
_cod_original_sg_symbol_H-M      'R -3 m H'
_cod_original_formula_sum        'Ba.98 Fe5.905 O11 Zn.94'
_cod_database_code               1008690
Low-temperature studies of two Y-type hexagonal ferrites: Ba Zn Fe6 O11 and Ba Co Fe6 O11
Collomb, A; Muller, J; Argoud, R; Journal of Magnetism and Magnetic Materials 130 (1994) 367–376; doi:10.1016/0304-8853(94)90696-3

data_1008691
_publ_section_title
;
Low-temperature studies of two Y-type hexagonal ferrites: Ba Zn Fe6 O11
and Ba Co Fe6 O11
;
_journal_coden_ASTM              JMMMDC
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              367
_journal_page_last               376
_journal_paper_doi               10.1016/0304-8853(94)90696-3
_journal_volume                  130
_journal_year                    1994
_chemical_formula_structural     'Ba0.96 Co0.985 Fe6.015 O11'
_chemical_formula_sum            'Ba0.96 Co0.985 Fe6.015 O11'
_chemical_name_systematic        'Barium cobalt iron(III) oxide (1/1/6/11)'
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   5.851(1)
_cell_length_b                   5.851(1)
_cell_length_c                   43.45399(200)
_cell_volume                     1288.3
_refine_ls_R_factor_all          0.092
_cod_original_sg_symbol_H-M      'R -3 m H'
_cod_original_formula_sum        'Ba.96 Co.985 Fe6.015 O11'
_cod_database_code               1008691
Etude des proprietes structurales et electriques de la solution solide Pb1-x Bix Ox F2-x
Soubeyroux, J L; Matar, S F; Reau, J M; Hagenmuller, P; Solid State Ionics 14 (1984) 337–345; doi:10.1016/0167-2738(84)90118-8

data_1008692
_publ_section_title
;
Etude des proprietes structurales et electriques de la solution solide
Pb1-x Bix Ox F2-x
;
_journal_coden_ASTM              SSIOD3
_journal_name_full               'Solid State Ionics'
_journal_page_first              337
_journal_page_last               345
_journal_paper_doi               10.1016/0167-2738(84)90118-8
_journal_volume                  14
_journal_year                    1984
_chemical_formula_structural     '(Pb.9 Bi.1) (O.1 F1.9)'
_chemical_formula_sum            'Bi0.1 F1.9 O0.1 Pb0.9'
_chemical_name_systematic        'Lead bismuth oxide fluoride (.9/.1/.1/1.9)'
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.937
_cell_length_b                   5.937
_cell_length_c                   5.937
_cell_volume                     209.3
_refine_ls_R_factor_all          0.013
_cod_original_formula_sum        'Bi.1 F1.9 O.1 Pb.9'
_cod_database_code               1008692